ASTM A928 / A928M – 11 Standard Specification for Ferritic/Austenitic (Duplex) Stainless Steel Pipe Electric Fusion Welded with Addition of Filler Metal
ASTM A928 standard specification covers standard requirements for ferritic/austenitic (duplex) stainless steel pipe that is electric fusion welded with addition of filler metal suitable for corrosive service. Heat treatment shall be performed after welding and in accordance with specified temperature and quench conditions. Several grades of ferritic/austenitic steel shall conform to the requirements of the applicable specification and grade designation. Heat and product analyses shall be conducted and shall conform to the requirements for the particular grade. The plate used in making the pipe shall conform to the required tensile properties. The steel pipe shall undergo several mechanical tests including transverse tension test, transverse guided-bend test, nondestructive test, hydrostatic test, and nondestructive electric test.
ASTM A928 Standard is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers electric-fusion-welded steel pipe suitable for corrosive service.
Note 1—The dimensionless designator NPS (nominal pipe size) has been substituted in this specification for traditional terms such as nominal diameter, size, and nominal size.
1.2 This specification covers grades of ferritic/austenitic steel as indicated in Table 1. The selection of the proper alloy and requirements for heat treatment shall be at the discretion of the purchaser, dependent on the service conditions to be encountered.
1.3 Five classes of pipe are covered as follows:
1.3.1 Class 1—Pipe shall be double welded by processes using filler metal in all passes and shall be radiographed completely.
1.3.2 Class 2—Pipe shall be double welded by processes using filler metal in all passes. No radiograph is required.
1.3.3 Class 3—Pipe shall be single welded by processes using filler metal in all passes and shall be radiographed completely.
1.3.4 Class 4—Same as Class 3, except that the weld pass exposed to the inside pipe surface is permitted to be made without the addition of filler metal (see 22.214.171.124 and 126.96.36.199).
1.3.5 Class 5—Pipe shall be double welded by processes using filler metal in all passes and shall be spot radiographed.
1.4 Supplementary requirements covering provisions ranging from additional testing to formalized procedures for manufacturing practice are provided. Supplementary Requirements S1 through S4 are included as options to be specified in the purchase order when desired.
1.5 The values stated in either SI units or inch-pound units are to be regarded separately as standard. Within the text, the SI units are shown in brackets. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard. The inch-pound units shall apply unless the M designation of the specification is specified in the order.